4076 Afr. J. Biotechnol. -1negative effect on quality of food or other packed materials according to ASTM E 1252-07.The samples were scanned at 4 cm(Raj, 2003). Also, starch based plastic did not have a resolution.negative effect on the environment and also reduced thegreen house effect (Bastioli, 2001). Synthetic plastic takes a Scanning electron microscope (SEM)long time to degrade in nature. The use of starch as abiodegradable agent accelarated the time of degradation Surface of blends was observed by Oxford Instruments INKA Pentain the environment. FET×3 scanning electron microscope at a voltage of 20 KV. Samples were fractured in liquid nitrogen, and then sputter was coated with gold.MATERIALS AND METHODSMaterials RESULTS AND DISCUSSIONLow Density Polyethylene (LDPE), with commercial grade (0200) Soil degradationwas prepared from Bandar Imam petrochemical complex, Iran.Food grade potato starch was obtained from Alvand co. Iran. Figure 1 shows the degradation of LDPE and LDPE/Glycerol with food grade was obtained from Merck co. Germany. potato starch in the soil. Plastic strips were buried in soilPolyethylene grafted maleic anhydride (PE-g- Ma) was produced inKarankin Co., Iran. Olive oil was used as a moisturizer. that consisted of compost, municipal waste, garden soil and P. aeruginosa; as an extra decomposer, that soil combination was a simulation of landfills. SoilCompounding environ-ment contains different kind of microorganism and macroorganisms. Weight losses of polymer strips in theStarch powder was plasticized with 25 wt% glycerol at 180°C for 10min. Samples were processed in HBI system (Haake Buchler soil could be assumed as an indicator of biodegradation inCompany from UK) with 60 rpm in 160°C. Sample sheets (0.4 mm the landfills or natural environment. Soil micro-organismsthickness) were prepared by using Hot Mini Press. attacked the polymer strips. First of all, microorganisms were attracted to the potato starch content of blends. Microorganisms consumed potato starch in the polymerPreparation of mould growth matrix and caused a fracture in the LDPE chain. BecauseThe suspension was prepared in distilled water with 0.05% dioctyl of the existence of maleic anhydride that made a chemicalsodium sulphosuccinate. Spore solution was put in sterile Petri bond between LDPE and potato starch, degradation ofdish. The polymer samples were immersed into suspension and potato starch caused a fracture in the polymer matrix andthen transferred to another sterile Petri dish and incubated in humidity biodegradation of LDPE. Figure 2 shows a Fouriergreater than 90 at 30°C for 84 days. According to standards, 8 transform spectroscopy (FTIR) confirming thekinds of mould species that included Aspergillus niger, Aspegillusterreus, Aureobasidium pullulans, Poecilomyces variotii, Penicillium biodegradation in soil environment and the FTIRfuniculosum, Penicillium ochrochloron, Scopulariopsis brevicaulis spectroscopy before and after degradation in soil.and Trichoderma viride were used for test. FTIR exhibited some change in LDPE/potato starch after degradation in soil. The highest decrease in spectrum was -1 observed at 1700 cm derived from carbonyl groups ofPreparation of bacterial growth potato starches. This reduction confirmed theFlat parts of polymer samples were cut into a square of 5 × 5 cm degra-dation of LDPE/potato starch in soil. Maleicand placed on the surface of the nutrient agar in the Petri dish. anhydride improved compatibility between non-polarPseudomonas aeroginosa was cultured on nutrient agar medium in LDPE and polar potato starches (Wang et al., 2005).sterile condition. A bacterial suspension was prepared in the -1 Absorption band was between 1081- 1089 cm because ofphysiological saline and then sprayed on the samples. A piece of the weak hydrogen bond between starch and glycerol.parafilm with dimensions of 4 × 4 was placed on it and was then -1incubated in humidity greater than 90 at 30°C for 84 days. Absorption band between 1081 and 1156 cm was derived from C-O-H stretching bond. Alcohol absorption band was -1 1070 – 1200 cm and this indicated a fast degradation rateSoil degradation of carbon chain (Labuzek et al., 2004).Samples were cut in strip shape and buried into soil for 8 months.The soil was a combination of P. aeruginosa, garden soil, leaf soil,compost and humus with bird fertilizer. FTIR test was performed on Exposure to P. aeroginosaeach sample before and after the soil was buried to confirm thebiodegradability in soil environment. Before and after the degradation test by bacteria, polymer samples were weighted. Table 1 shows the percentages of polymer weight loss during degradation by P. aeroginosa.Fourier transform spectroscopy (FTIR) Accordingly, pure LDPE had a little weight loss. The weightThis test was performed using equinox 55 made by Bruker at 23°C. loss could be attributed to biodegradationThe diameter of samples was 0.4 mm and the test wasrun
Borghei et al 4077 Time(months) Figure 1. Weight loss of polymeric samples during 8 months soil burial. Figure 2. Fourier transform spectroscopy (FTIR) of potato starch based LDPE (LDPE/potato starch) before and after degradation in soil. Table 1. Weight change of potato starch based LDPE after 84 significant weights loss. It days exposure to P. aeruginosa. Samples Weight lose (%)LDPE 0.43LDPE/ potato starches 2.19by P. aeroginosa, because carbon free media coulddegrade low density polyethylene (Agamuthuand Faizura, 2005). LDPE/potato starch showed
was determined that potato starches were the only sourceof carbon for microorganisms. As shown in Figure 3 part(b), black spot appeared on the surface of samples, whichindicate the bacterial growth; but pure LDPE did not showany visible growth. To ensure bacterial degradation, SEM test was done.Figures 4 and 5 display the scanning electron micrographof pure LDPE and LDPE/potato starches blend after 84days’ incubation by P. aeroginosa. Scanning electronmicrograph (SEM) confirmed the observation of bacterialgrowth and weights loss measurement. According toFigure 4, the surface of LDPE was smooth. As it is shown
4078 Afr. J. Biotechnol. a b Figure 3. LDPE/potato starch before (a) and after (b) 84 days of exposure to P. aeroginosa. Figure 4. Scanning electron micrograph of LDPE after 84 days of exposure to P. aeroginosa. Figure 5. Scanning electron micrograph of potato starch based LDPE after 84 days of exposure to P. aeroginosa.in Figure 5, some holes and bores appeared on the lead to accelerated LDPE biodegradation. Thesesurface of the LDPE/potato starch blend. These holes obser-vations agreed with other researchesindicate the rate of biodegradation and confirmed the (Rantanakamnuan and Aht-Ong, 2006).potato starches removal by P. aeroginosa function. Boresshow the area attacked by microorganisms. Potato starchwas used as a main source of nutrient by P. aeroginosa. Fungi growthPotato starch consumption by bacteria caused holes in thepolymer matrix and eventually the degradation of the After 20 days of sample incubation, 20% of Petri dishespolymer. Because polyethylene grafted maleic anhydride were covered by fungi growth. Samples were colonized bymade a chemical bond between potato starch and mould about 50% in the middle of the incubation period.polyethylene backbone, biodegradation of potato starch Fungi colonized potato starch/LDPE surface more
Borghei et al 4079 Table 2. Visual examination of LDPE/ Potato starch blends during incubation. Cultivation time (days) LDPE LDPE/ Potato starch 20 0 2 40 0 3 84 0 3 0 = No apparent growth under a nominal magnification of approximately 50×. 2 = Growth plainly visible to the naked eye, but covers less than 25% of the test surface. 3 = Growth plainly visible to the naked eye and covering more than 25% of the test surface. confirmed the microbial degradability of potato starch based LDPE. Scanning electron micrograph (SEM) after exposure to P. aeroginosa confirmed the potato starch Figure 6. Visual fungal growth on LDPE/potato starch blend after 84 removal of LDPE/potato starch blend. Existence of days incubation. anhydride maleic created linkage between LDPE and potato starch, so consumption of potato starch in any environment caused a destruction of polymer matrix. Consumption of potato starch as a biodegradable agentthan 80% at the end of the incubation as shown in Figure initiates the biodegradation process. According to this6. After 84-days of incubations, LDPE strips did not exhibit research, potato starch based low density polyethylene iscolor change or mould growth. This result is similar to other a microbial biodegradable polymer.researchers’ work on polymer degradation (Abdolrahmanet al., 2006). Table 2 shows the fungal growth rate on thesamples. As shown in Figure 4, more than 80% of samples REFERENCESwere covered by mould growth. Genus Penicillum could decompose hazardous materials Abdolrahman W, Rasit A, Zakaria N (2006). Studies onand plastic (brukato and Wong, 1991). Genus Aspergillus Biodegradability, Morphology and Mechanical Properties of Lowis described as a decomposer of polyethylene, DDT and Density Polyethylene/Sago Based Blends. 1ststarches (Labuzek et al., 2004; Scherer et al., 1999). InternationalPotato starch in polymer blends had a digestible link for Conference on Natural Resources Engineering & Technology,mould and fungi. Microorganisms recognized the potato Putrajaya, Malaysia, pp. 434-444. Agamuthu P, Faizura PN (2005)starch carbon link as a nutrient source. Consumption of Biodegradability of degradable plasticpolar hydrophilic starch caused fracture in the polymer waste. Waste Manage. Res. 23(2): 95-100. Bastioli C (2001). Globalchain. Maleic anhydride created a link between two status of the production of biobased packaging materials. Starch/Stärke. 53: 351-355. Breslin VT (1993). Degradationincompatible particles, so with starch removal, a gap of starch-based plastic composites in aappeared in the polymer chain. Through the gap, municipal solid waste landfills. J. Polymer Environ. 1(2): 127-141.microorganism’s had access to the carbon link of Brukato CL, Wong SS (1991). Extracellular poly (3-hydroxybutyrate)polyethylene; the result is the polymer biodegradation. depolymerase from Penicillum funiculosum general characteristics and Active Site Studies. Arch. Biochem. Biophys. 290(2): 497-592. Chiellinia E, Corti A, Swift G (2003). Biodegradation of thermally oxidized, fragmented low density polyethylene. Polymer degradationConclusion and stability, 81: 341-351. Labuzek S, Nowak B, Pajak J (2004). The Susceptibility of Polyethylene Modified with Bionolle to Biodegradation by Filamentous Fungi; Pol.Growing concern about environment pollution leads to J. Environ. Stud. 13 (1): 59-68. Labuzek S, Nowak B, Pajak J (2004).public trends usage of biodegradable polymers. Natural The susceptibility of Polyethylenepolymers were used as a biodegradable additive. In this Modified with Bionolle to Biodegradation by Filamentous Fungi. Pol J.work, potato starch was a selected biopolymer. Microbial Environ. Stud. 13(1): 59-68. Labuzek S, Nowak B, Pajak J (2004). The Susceptibility of Polyethylenebiodegradation of potato starch based on low density Modified with Bionolle to Biodegradation by Filamentous Fungi; Pol.polyethylene was examined under natural and laboratory J. Environ. Stud. 13(1): 59-68. Matzinos P, Bikiaris D, Kokkou S,condition. Potato starch/LDPE weight loss and FTIR test Panayiotou C (2001). Processing andafter the soil was buried were stimulated as biodegradation Characterization of LDPE/Starch Products. J. Appl. Polymer Sci. 79:in landfills. Microbial degradation in laboratory by 8 kinds 2548-2557. Ojumo TV, Yu J, Solomon BO (2004). Production ofof fungi and exposure to P. aeroginosa was done and this Polyhydroxyalkanoates, a bacterial biodegradable polymer. Afr. J. Biotechnol. 3(1): 18-24. Raj B, Sankar U (2004). LLDPE/Starch blend films for food packaging
applications. Adv. Polymer Technol. 23(1): 32-45.
4080 Afr. J. Biotechnol.Rantanakamnuan U, Aht-Ong D (2006). Photobiodegradation of low Wang S, Yu J, Yu J (2005). Compatible thermoplastic starch/polyethylene density polyethylene/ banana starch films; J. Appl. Polymer Sci. 100: blends by one-step reactive extrusion; Polym. Int. 54: 279-285. 2725-2736.Rutkowska M, Heimowska A, Krasowska K, Janik H (2002). Biodegradability of Polyethylene Starch Blends In Sea Water. Pol. J. Environ. Stud. 11(3): 267-274.Scherer TM, Fuller RC, Lenz RW, Goodwin S (1999). Hydrolase activity of an extracellular depolymerase from Aspergillus fumigatus with bacterial and synthetic polyesters. Polym. Degrad. Stab. 64: 267-275.